Ni3Cl2.1(OH)3.9·4H2O, the Ni Analogue to Mg3Cl2(OH)4·4H2O.
Bette, Sebastian; Dinnebier, Robert E.; Freyer, Daniela; Inorganic chemistry 53 (2014) 4316–4324; doi:10.1021/ic500251x

data_4338187
_publ_section_title
;
 Ni3Cl2.1(OH)3.9&#x00B7;4H2O, the Ni Analogue to Mg3Cl2(OH)4&#x00B7;4H2O.
;
_journal_issue                   9
_journal_name_full               'Inorganic chemistry'
_journal_page_first              4316
_journal_page_last               4324
_journal_paper_doi               10.1021/ic500251x
_journal_volume                  53
_journal_year                    2014
_chemical_formula_moiety         'Cl2.1 H11.9 Ni3 O7.9'
_chemical_formula_sum            'Cl2.1 H11.9 Ni3 O7.9'
_chemical_formula_weight         388.909
_chemical_name_common            'Ni 1.95-1.05-4; 1.95 Ni(OH)2 1.05NiCl2 4H2O'
_space_group_IT_number           12
_symmetry_Int_Tables_number      12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_audit_creation_method           TOPAS
_cell_angle_alpha                90
_cell_angle_beta                 101.5675(23)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.95746(39)
_cell_length_b                   3.14125(11)
_cell_length_c                   10.48180(49)
_cell_measurement_temperature    295
_cell_volume                     482.49(3)
_diffrn_ambient_temperature      295
_diffrn_detector
; 
 Mythen Dectris 1 K  
;
_diffrn_radiation_monochromator
'Johannson Ge(111) primary beam monochromator'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.70930
_diffrn_source_type              Mo-tube
_exptl_absorpt_process_details
;   
 ?
;
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.67
_exptl_crystal_description       'microcrystalline powder'
_pd_calc_method                  'Rietveld Refinement'
_pd_instr_location
; 
'Stoe Stadi P, Debye-Scherrer mode, MPI-FKF, Stuttgart, Germany'
;
_pd_meas_2theta_range_inc        0.012
_pd_meas_2theta_range_max        60.0
_pd_meas_2theta_range_min        2.0
_pd_meas_scan_method             step
_pd_proc_2theta_range_inc        0.012
_pd_proc_2theta_range_max        60.0
_pd_proc_2theta_range_min        2.0
_pd_proc_info_data_reduction     binning
_pd_proc_info_excluded_regions
;
 ?
;
_pd_proc_ls_background_function
;   
'Chebyshev polynomial'
;
_pd_proc_ls_peak_cutoff          0.00100
_pd_proc_ls_profile_function
;
 Fundamental parameters
;
_pd_proc_ls_prof_R_factor        0.0215
_pd_proc_ls_prof_wR_expected     0.0023
_pd_proc_ls_prof_wR_factor       0.0276
_pd_spec_mounting
; 
'0.5 mm glass capillary'
;
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_refine_ls_number_parameters     56
_refine_ls_R_Fsqd_factor         0.0073
_cod_data_source_file            ic500251x_si_001.cif
_cod_data_source_block           Ni214
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 4338187.cif.
;
_cod_original_cell_volume        482.486(31)
_cod_database_code               4338187